 # Lecture 4 The structure of crystalline solids L e a r n i n g O b j e c t i v es outcomes: 1.Describe the difference in atomic/molecular structure between.

## Presentation on theme: "Lecture 4 The structure of crystalline solids L e a r n i n g O b j e c t i v es outcomes: 1.Describe the difference in atomic/molecular structure between."— Presentation transcript:

Lecture 4 The structure of crystalline solids L e a r n i n g O b j e c t i v es outcomes: 1.Describe the difference in atomic/molecular structure between crystalline and noncrystalline materials. 2. Draw unit cells for face-centered cubic, body centered cubic, and hexagonal close-packed crystal structures. 3. Derive the relationships between unit cell edge length and atomic radius for face-centered cubic and body- centered cubic crystal structures. 4. Compute the densities for metals having face centered cubic and body-centered cubic crystal structures given their unit cell dimensions.

Fundamentals Concepts:  Crystalline: A crystalline material is one in which the atoms are situated in a repeating or periodic array over large atomic distances.  Crystal structure: Some of the properties of crystalline solids depend on the crystal structure of the material, the manner in which atoms, ions, or molecules are spatially arranged.  Lattice: lattice is used in the context of crystal structures; in this sense ‘‘lattice’’ means a three-dimensional array of points coinciding with atom positions (or sphere centers).

UNIT CELLS:  The atomic order in crystalline solids indicates that small groups of atoms form a repetitive pattern. Thus, in describing crystal structures, it is often convenient to subdivide the structure into small repeat entities called unit cells.  Thus, the unit cell is the basic structural unit or building block of the crystal structure and defines the crystal structure by virtue of its geometry and the atom positions within METALLIC CRYSTAL STRUCTURES:  Three relatively simple crystal structures are found for most of the common metals: face-centered cubic, body- centered cubic, and hexagonal close-packed.

THE FACE-CENTERED CUBIC CRYSTAL STRUCTURE:  The crystal structure found for many metals has a unit cell of cubic geometry, with atoms located at each of the corners and the centers of all the cube faces. It is aptly called the face-centered cubic (FCC) crystal structure.  Examples: Some of the familiar metals having this crystal structure are copper, aluminum, silver, and gold. Figure 3.1a shows a hard sphere model for the FCC unit cell, whereas in Figure 3.1b the atom centers are represented by small circles to provide a better perspective of atom positions. The aggregate of atoms in Figure 3.1c represents a section of crystal consisting of many FCC unit cells. These spheres or ion cores touch one another across a face diagonal; the cube edge length a and the atomic radius R are related through the following:

 Corner and face positions are really equivalent; that is, translation of the cube corner from an original corner atom to the center of a face atom will not alter the cell structure.  Two other important characteristics of a crystal structure are the coordination number and the atomic packing factor (APF).  The coordination number: For metals, each atom has the same number of nearest-neighbor or touching atoms, which is the coordination number. For face- centered cubics, the coordination number is 12. The APF is the fraction of solid sphere volume in a unit cell, assuming the atomic hard sphere model, or the following:

 For the FCC structure, the atomic packing factor is 0.74, which is the maximum packing possible for spheres all having the same diameter. Computation of this APF is also included as an example problem. Metals typically have relatively large atomic packing factors to maximize the shielding provided by the free electron cloud.

THE BODY-CENTERED CUBIC CRYSTAL STRUCTURE: Another common metallic crystal structure also has a cubic unit cell with atoms located at all eight corners and a single atom at the cube center. This is called a body- centered cubic (BCC) crystal structure. A collection of spheres depicting this crystal structure is shown in Figure 3.2c, whereas Figures 3.2a and 3.2b are diagrams of BCC unit cells with the atoms represented by hard sphere and reduced-spheren models, respectively. Center and corner atoms touch one another along cube diagonals, and unit cell length a and atomic radius R are related through.:

 Chromium, iron, tungsten, as well as several other metals listed in Table 3.1 exhibit a BCC structure. Two atoms are associated with each BCC unit cell: the equivalent of one atom from the eight corners, each of which is shared among eight unit cells, and the single center atom, which is wholly contained within its cell. In addition, corner and center atom positions are equivalent. The coordination number for the BCC crystal structure is 8; each center atom has as nearest neighbors its eight corner matoms. Since the coordination number is less for BCC than FCC, so also is the atomic packing factor for BCC lower—0.68 versus 0.74.

THE HEXAGONAL CLOSE-PACKED CRYSTAL STRUCTURE  Not all metals have unit cells with cubic symmetry; the final common metallic crystal structure to be discussed has a unit cell that is hexagonal. Figure 3.3a shows a reduced-sphere unit cell for this structure, which is termed hexagonal close-packed (HCP); an assemblage of several HCP unit cells is presented in Figure 3.3b.  The top and bottom faces of the unit cell consist of six atoms that form regular hexagons and surround a single atom in the center. Another plane that provides three additional atoms to the unit cell is situated between the top and bottom planes. The atoms in this midplane have as nearest neighbors atoms in both of the adjacent two planes.  The equivalent of six atoms is contained in each unit cell; one- sixth of each of the 12 top and bottom face corner atoms, one- half of each of the 2 center face atoms, and all the 3 midplane interior atoms. If a and c represent, respectively,

 The short and long unit cell dimensions of Figure 3.3a, the c/a ratio should be 1.633; however, for some HCP metals this ratio deviates from the ideal value. The coordination number and the atomic packing factor for the HCP crystal structure are the same as for FCC: 12 and 0.74, respectively.  The HCP metals include cadmium, magnesium, titanium, and zinc; some of these are listed in Table 3.1.

Download ppt "Lecture 4 The structure of crystalline solids L e a r n i n g O b j e c t i v es outcomes: 1.Describe the difference in atomic/molecular structure between."

Similar presentations